Correlated-Electron Systems and High-Temperature
Takashi Yanagisawa1, Mitake Miyazaki2, Kunihiko Yamaji1
1Electronics and Photonics Research Group, National Institute of Advanced Industrial Science and Technology (AIST), Tsukuba Central 2, Tsukuba, Japan
2Hakodate National College of Technology, Hakodate, Japan Email: email@example.com
Received April 2, 2013; revised May 5, 2013; accepted June 1,2013
Copyright © 2013 Takashi Yanagisawa et al. This is an open access article distributed under the Creative Commons Attribution Li- cense, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
We present recent theoretical results on superconductivity in correlated-electron systems, especially in the two- dimensional Hubbard model and the three-band d-p model. The mechanism of superconductivity in high-temperature superconductors has been extensively studied on the basis of various electronic models and also electron-phonon models. In this study, we investigate the properties of superconductivity in correlated-electron systems by using numerical methods such as the variational Monte Carlo method and the quantum Monte Carlo method. The Hubbard model is one of basic models for strongly correlated electron systems, and is regarded as the model of cuprate high temperature superconductors. The d-p model is more realistic model for cuprates. The superconducting condensation energy obtained by adopting the Gutzwiller ansatz is in reasonable agreement with the condensation energy estimated for YBa2Cu3O7. We show the phase diagram of the ground state using this method. We have further investigated the stability of striped and checkerboard states in the under-doped region. Holes doped in a half-filled square lattice lead to an incommensurate spin and charge density wave. The relationship of the hole density x and incommensurability ,
, is satisfied in the lower doping region, as indicated by the variational Monte Carlo calculations for the two-dimensional Hubbard model. A checkerboard-like charge-density modulation with a roughly 4 4 period has also been observed by scanning tunneling microscopy experiments in Bi2212 and Na-CCOC compounds. We have performed a variational Monte Carlo simulation on a two-dimensional t-t-t-U Hubbard model with a Bi-2212 type band structure and found that the 4 4 period checkerboard spin modulation, that is characterized by multi Q vectors, is indeed stabilized. We have further performed an investigation by using a quantum Monte Carlo method, which is a numerical method that can be used to simulate the behavior of correlated electron systems. We present a new algorithm of the quantum Monte Carlo diagonalization that is a method for the evaluation of expectation value without the negative sign problem. We compute pair correlation functions and show that pair correlation is indeed enhanced with hole doping.
Keywords: High-Temperature Superconductivity; Strongly Correlated Electrons; Monte Carlo Methods; Hubbard
Model; Condensation Energy; Pair-Correlation Function
The effect of the strong correlation between electrons is important for many quantum critical phenomena, such as unconventional superconductivity (SC) and the metal- insulator transition. Typical correlated electron systems are high-temperature superconductors [1-5], heavy fer- mions [6-9] and organic conductors . The phase diagram for the typical high-Tc cuprates is shown in
Figure 1 . It has a characteristics that the region of
antiferromagnetic order exists at low carrier concentra-
tions and the superconducting phase is adjacent to the antiferromagnetism.
In the low-carrier region shown in Figure 2, there is
the anomalous metallic region where the susceptibility and 1T1 show a peak above Tc suggesting an existence of the pseudogap. To clarify an origin of the anomalous metallic behaviors is also a subject attracting many physicists as a challenging problem.
It has been established that the Cooper pairs of high-Tc
Figure 1. Phase diagram delineating the regions of super- conductivity and antiferromagnetic ordering of the Cu2+ ions for the hole-doped La2–xSrxCuO4 and electron-doped
Figure 2. Phase diagram showing the regions of non-Fermi liquid and pseudogap metal for the hole-doped case. The boundaries indicated in the figure are not confirmed yet.
symmetry were provided for the electron-doped cuprates Nd2–xCexCuO4 [13-15]. Thus it is expected that the superconductivity of electronic origin is a candidate for the high-Tc superconductivity. We can also expect that the origin of d-wave superconductivity lies in the on- site Coulomb interaction of the two-dimensional Hub- bard model.
The antiferromagnetism should also be examined in correlated electron systems. The undoped oxide com- pounds exhibit rich structures of antiferromagnetic cor- relations over a wide range of temperature that are described by the two-dimensional quantum antiferro- magnetism [16-18]. A small number of holes introduced by doping are responsible for the disappearance of long-range antiferromagnetic order [19-24].
Recent neutron scattering experiments have suggested an existence of incommensurate ground states with modulation vectors given by Qs
Q (or Qs
Q ) where denotes the hole-doping ratio . We can expect that the incommensurate cor-
relations are induced by holes doped into the Cu-O plane in the underdoped region. A checkerboard-like charge-density modulation with a roughly 4 4 pe- riod has also been observed by scanning tunneling microscopy experiments in Bi2212 and Na-CCOC com- pounds.
Recently the mechanism of superconductivity in high- temperature superconductors has been extensively stu- died using various two-dimensional (2D) models of electronic interactions. Among them the 2D Hubbard model  is the simplest and most fundamental model. This model has been studied intensively using numerical tools, such as the Quantum Monte Carlo method [27-42], and the variational Monte Carlo method [24,43-50]. The two-leg ladder Hubbard model was also investigated with respect to the mechanism of high-temperature supercon- ductivity [51-59].
Since the discovery of cuprate high-temperature su- perconductors, many researchers have tried to explain the occurrence of superconductivity of these materials in terms of the two-dimensional (2D) Hubbard model. However, it remains matter of considerable controversial as to whether the 2D Hubbard model accounts for the properties of high-temperature cuprate superconductors. This is because the membership of the the two-dimen- sional Hubbard model in the category of strongly correlated systems is a considerable barrier to progress on this problem. The quest for the existence of a superconducting transition in the 2D Hubbard model is a long-standing problem in correlated-electron physics, and has been the subject of intensive study [35,36,38,46, 60,61]. In particular, the results of quantum Monte Carlo methods, which are believed to be exact unbiased me- thods, have failed to show the existence of super- conductivity in this model [38,61].
In the weak coupling limit we can answer this question. We can obtain the superconducting order parameter of the Hubbard model in the limit of small U, that is given by [62-66]
where U is the strength of the on-site Coulomb interaction and the exponent x is determined by solv- ing the gap equation. Thus the existence of the super- conducting gap is guaranteed by the weak coupling theory although is extremely small because of the exponential behavior given above. x indicates the strength of superconductivity. In the intermediate or large coupling region, we must study it beyond the perturbation theory.
obtained by using the quantum variational Monte Carlo method. The superconducting condensation energy ob- tained by adopting the Gutzwiller ansatz is in reasonable agreement with the condensation energy derived for YBa2Cu3O7. We have further investigated the stability of striped and checkerboard states in the under-doped region. Holes doped in a half-filled square lattice lead to an incommensurate spin and charge density wave. The relationship of the hole density x and incommensurability
, x, is satisfied in the lower doping region. This is consistent with the results by neutron scattering measurements. To examine the stability of a 4 4
checkerboard state, we have performed a variational Monte Carlo simulation on a two-dimensional
t t t U Hubbard model with a Bi-2212 type band structure. We found that the 4 4 period checkerboard checkerboard spin modulation that is characterized by multi Q vectors is stabilized.
Further investigation has been performed by using the quantum Monte Carlo method which is a numerical method that can be used to simulate the behavior of correlated electron systems. This method is believed to be an exact unbiased method. We compute pair cor- relation functions to examine a possibility of super- conductivity.
The Quantum Monte Carlo (QMC) method is a numerical method employed to simulate the behavior of correlated electron systems. It is well known, however, that there are significant issues associated with the application to the QMC. First, the standard Metropolis (or heat bath) algorithm is associated with the negative sign problem. Second, the convergence of the trial wave function is sometimes not monotonic, and further, is sometimes slow. In past studies, workers have inves- tigated the possibility of eliminating the negative sign problem [37,38,40-42]. We present the results obtained by a method, quantum Monte Carlo diagonalization, without the negative sign problem.
2. Hubbard HamiltonianThe Hubbard Hamiltonian is
ij i i i i
t c c U
n n (2)
c and ci denote the creation and annihilation
operators of electrons, respectively, and †
i i i
n c c is the number operator. The second term represents the on-site Coulomb interaction which acts when the two electrons occupy the same site. The numbers of lattice sites and electrons are denoted as N and Ne ,
respectively. The electron density is neN Ne .
In the non-interacting limit U0, the Hamiltonian is easily diagonalized in terms of the Fourier transformation. In the ground state each energy level is occupied by
electrons up to the Fermi energy. In the other limit 0
t , each site is occupied by the up- or down-spin electron, or is empty. The non-zero tij induces the
movement of electrons that leads to a metallic state id
N N . The ground state is probably insulating at half-filling NeN if U is sufficiently large.
If tij t are non-zero only for the nearest-neighbor
pairs, the Hubbard Hamiltonian is transformed to the following effective Hamiltonian for large U t :
† † †
† † † †
† † ,
i j j j j
j j j j j j j j
j j j j
H t a a a a a a
a a a a a a a a
a a a a
where ai ci
and j and j in-
dicate the nearest-neighbor sites in the and directions, respectively. The second term contains the three-site terms when . If we neglect the three-site terms, this effective Hamiltonian is reduced to the t-J model:
i j i j i j
H t a a J n n
where J4t U2 .
The Hubbard model has a long history in describing the magnetism of materials since the early works by Hubbard , Gutzwiller  and Kanamori . One- dimensional Hubbard model has been well understood by means of the Bethe ansatz [70-72] and conformal field theory [73-75]. The solutions established a novel concept of the Tomonaga-Luttinger liquid  which is described by the scalar bosons corresponding to charge and spin sectors, respectively. The correlated electrons in two- and three-dimensional space are still far from a complete understanding in spite of the success for the one-di- mensional Hubbard model. A possibility of supercon- ductivity is a hot topic as well as the magnetism and metal-insulator transition for the two- and three-di- mensional Hubbard model.
The three-band Hubbard model that contains d and
p orbitals has also been investigated intensively with respect to high temperature superconductors [24,64, 77-88]. This model is also called the d-p model. The 2D three-band Hubbard model is the more realistic and relevant model for two-dimensional CuO2 planes which are contained usually in the crystal structures of high-Tc
superconductors. The network of CuO2 layer is shown in
Figure 3. The parameters of the three-band Hubbard
model are given by the Coulomb repulsion Ud, energy
levels of p electrons p and d electron d, and
transfer between p orbitals given by tpp. Typical
Figure 3. The lattice of the three-band Hubbard model on the CuO2 plane. Small circles denote Cu sites and large ones
denote O sites.
Table 1. Typical parameter values for the three-band Hub- bard model. Energies are measured in eV.
Ref. Ref. Ref. Ref.
3.6 2.75 - 3.75 3.5 2.5
t 1.3 1.5 1.5 1.47
t 0.65 0.65 0.6
U 10.5 8.8 9.4 9.7
U 4.0 6.0 4.7 5.7
U 1.2 <1.0 0.8 <1
three-band Hubbard model is written as [24,47,48,80] (see Equation (4)) where ˆx and ˆy represent unit vectors along x and y directions, respectively. †
ˆ 2, i x
ˆ 2, i x
p denote the operators for the p electrons at site
R x . Similarly † ˆ 2, i y
p and pi yˆ 2, are defined.
U denotes the strength of Coulomb interaction between
d electrons. For simplicity we neglect the Coulomb interaction among p electrons in this paper. Other notations are standard and energies are measured in tdp
units. The number of cells is denoted as N for the three-band Hubbard model. In the non-interacting case
the Hamiltonian in the k-space is written as (see Equation (5)).
dk , pxk
pk and pyk
y p k are operators for d -, px- and py -electron of the
momentum k and spin , respectively.
In the limit tdpUd
, tdppd, and p d Ud
, the d- p model is mapped to the t-J
2 1 2
d p d p
J t U U (6)
eff dp p d
t t . JK 4teff gives the
antiferromagnetic coupling between the neighboring d
and p electrons. In real materials
tdp is not
so large. Thus it seems that the mapping to the t-J model is not necessarily justified.
3. Variational Monte Carlo Studies
In this Section we present studies on the two-dimensional Hubbard model by using the variational Monte Carlo method.
3.1. Variational Monte Carlo Method
Let us start by describing the method based on the 2D Hubbard model. The Hamiltonian is given by
† † h.c. h.c. , i j ij
j j j
H t c c
t c c U n n
where ij denotes summation over all the nearest- neighbor bonds and j means summation over the next nearest-neighbor pairs. t is our energy unit. The dispersion is given by
2 cost kx cos ky 4 cost kx cos ky .
Our trial wave function is the Gutzwiller-projected wave functions defined as
n P PN G
s P PN G BCS
† † † † †
ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2, †
ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2,
† † †
ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2 h.c.
dp d i i d i i i i p i x i x i y i y
i i i
dp i i x i y i x i y
pp i y i x i y i x i y i x
H d d U d d d d p p p p
t d p p p p
t p p p p p p
† ˆ ˆ
, i y/ 2, i x/ 2, h.c. . i p p
0 ? † †
2i sin 2 h.c.
2i sin 2 h.c. 4 sin 2 sin 2 h.c. ,
dp d p x x y y dp x x
dp y y pp x y x y
H d d p p p p t k d p
t k d p t k k p p
k k k k k k k k
k k k
k k k k
where † 0 , 0 , F k c
BCS u v c c
k k k k k
P is the Gutzwiller projection operator given by
1 1 ;
G j j
g n n (13)
g is a variational parameter in the range from 0 to unity and j labels a site in the real space. PNe is a pro-
jection operator which extracts only the sites with a fixed total electron number Ne. Coefficients uk and vk in
appear in the ratio defined by
k k k
where kk and k is a k-dependent gap func- tion. is a variational parameter working like the chemical potential. ck is the Fourier transform of cj.
The wave functions n and s are expressed by the Slater determinants for which the expectations values are evaluated using a Monte Carlo procedure [43,44,92]. s is written as
† † † † 2 † † exp 0
exp , 0
, 0 ,
s N G
N G j
P P v u c c
P P a j c c
P a j c c
k k k k
k (15) where
a j N
v uk k i
k R R
Then s is written using the Slater determinants as
1 2 1 2
1 2 2 1 2 2
1 2 1 2
† † † † † †
, 0 ,
s G N N
j j j
P A j i
c c c c c c
where A j
1iNe2, 1 Ne 2
is the Slater determinant defined by
1 1 1 2 1 2
2 1 2 2 2 2
2 1 2 2 2 2
, , , , , , . , , , e e e
e e e e
N N N N
a j a j a j
a j a j a j
a j a j a j
In the process of Monte Carlo procedure the values of cofactors of the matrix in Equation (18) are stored and corrected at each time when the electron distribution is modified. We optimized the ground state energy
g s s s s
E H H (19) with respect to g, k and for s for s. For
the variational parameter is only g . We can employ the correlated measurements method  in the process of searching optimal parameter values mini- mizing Eg.
A Monte Carlo algorithm developed in the auxiliary field quantum Monte Carlo calculations can also be employed in evaluating the expectation values for the wave functions shown above [94-96]. Note that the Gutzwiller projection operator is written as
G i i
i P n n
(20) where log 1
g . Then using the discrete Hubbard- Stratonovich transformation, the Gutzwiller operator is the bilinear form:
1 2 exp 2 ,
i i i i
i i i i i
s i i
a s n n n n
(21) where cosh 2
a e2. The Hubbard-Stratonovich au- xiliary field si takes the values of 1. The norm
is written as
† 0 0
const det exp ,
exp , ,
i i n n u s V u V s
s, is a diagonal N N matrix corre- sponding to the potential
i i i
h s a s n n
V s is written as
, diag 2
1 2, ,2 N 2,0,
V s a s a s (24) where diag ,
denotes a diagonal matrix with ele- ments given by the arguments a,. The elements of
i1, , ; N j1, , Ne 2
are given by linear combinations of plane waves. For example,
0 ij exp
method is used to consider an off-diagonal Jastrow cor- relation factor of exp(–S)-type. The results for the im- proved wave functions are discussed in Section 3.10.
3.2. Superconducting Condensation Energy
We study the cases of the d-, extended s- (s-) and
s-wave gap functions in the following:
cos x cos y ,
d k k k (26)
cos x cos y ,
s k k
s k (28) In Figure 4 calculated energies per site with Ne84
on the 10 10 lattice are shown for the case of U8 and t 0. E Ng is plotted as a function of
for three types of gap functions shown above. We impose the periodic and the antiperiodic boundary conditions for
x- and y-direction, respectively. This set of boundary conditions is chosen so that k does not vanish for any
k-points occupied by electrons. Eg was obtained as the
average of the results of several Monte Carlo calculations each with 5 10 7 steps.
E N has minimum at a finite value of 0.08 in the case of the d-wave gap function.
The energy gain Eg in the superconducting state is
called the SC condensation energy in this paper.
g E N
is plotted as a function of 1 N in Figure 5 in
order to examine the size dependence of the SC energy gain . Lattice sizes treated are from 8 8 to
22 22 . The electron density ne is in the range of
0.80ne0.86. Other parameters are 0.20 t 0.0 and U t8 in t units. Bulk limit N of SC condensation energy Econd was obtained by plotting as
a function of 1N. The linear fitting line indicates very
Figure 4. Ground state energy per site Eg N for the 2D Hubbard model is plotted against for the case of 84 electrons on the 10 × 10 lattice with U8 and t0 . Solid curves are for the d-wave gap function. Squares and triangles are for the s*- and s-wave gap functions, respectively. The diamond shows the normal state value .
Figure 5. Energy gain per site in the SC state with reference to the normal state for the 2D Hubbard model is plotted as a function of 1N. L is the length of the edge of the square lattice. YBCO attached to the vertical axis indicates the experimental value of the SC condensation energy for YBa2Cu3O4 .
clearly that the bulk limit remains finite when 0.25 t 0.10
and ne0.84 . When ne0.86 , 0.20
t and U8 , the bulk-limit Econd is 0.00117 site 0.60 meV site
E , where t = 0.51
eV is used . Thus the superconductivity is a real bulk property, not a spurious size effect. The value is re- markably close to experimental values 0.17 ~ 0.26 meV/site estimated from specific heat data [99,100] and 0.26 meV/site from the critical magnetic field Hc  for optimally doped YBa2Cu3O4 (YBCO). This good agreement strongly indicates that the 2D Hubbard model includes essential ingredients for the superconductivity in the cuprates.
We just point out that the t-J model gives = 0.026 13 meV site
E t at ne0.84 for J = 4
t2/U = 0.5 and t 0 . This value is 50 times larger than the experimental values indicating a serious quan- titative problem with this model. This means that the t-J
model made from the leading two terms in the expansion in terms of t U of the canonical transformation of the Hubbard model should be treated with the higher-order terms in order to give a realistic SC condensation ener- gy.
Here we show the SC condensation energy as a function of U in Figure 6. The condensation energy
E E N is increased as U t is increased as far as U t12. In the strong coupling region U8t, we obtain the large condensation energy.
3.3. Fermi Surface and Condensation Energy
Figure 6. Energy gain per site in the SC state with reference to the normal state for the 2D Hubbard model as a function of the Coulomb repulsion U. The system is 10 × 10 with the electron number Ne84 and t 0.3 .
for YBCO.  The band parameter values of LSCO were estimated as t 0.12 and t 0.08. This set corresponds roughly to Econd 0.0010. The latter value is much larger than the above-mentioned experi- mental value for LSCO. However, the stripe-type SDW state coexists with superconductivity [105,106] and the SC part of the whole Econd is much reduced. Therefore,
such a coexistence allows us to qualitatively understand the SC Econd in LSCO.
On the other hand, Tl2201
band calculations by Singh and Pickett 
give very much deformed Fermi surfaces that can be fitted by large t such as t 0.4. For Tl2201, an Angular Magnetoresistance Oscillations (AMRO) work  gives information of the Fermi surface, which allows to get t 0.2 and t0.165. There is also an Angle-Resolved Photoemission Study (ARPES) , which provides similar values. In the case of Hg1201, there is an ARPES work , form which we obtain by fitting t 0.2 and t0.175. For such a deformed Fermi surface, Econd in the bulk limit is reduced con- siderably. [111,112] Therefore, the SC Econd calculated
by VMC indicates that the Fermi surface of LSCO-type is more favorable for high Tc. The lower Tc in LSCO
may be attributed to the coexistence with antiferro- magnetism of stripe type.
3.4. Ladder Hubbard Model
The SC condensation energy in the bulk limit for the ladder Hubbard model has also been evaluated using the variational Monte Carlo method . The Hamiltonian is given by the 1D two-chain Hubbard model: [51,52,55, 56,85,113-116]
1 2 , 1,
ladder d j j
j j j j
H t c c t c c
U c c c c
where † j
cj is the creation (annihilation) operator of an electron with spin at the th site along the jth chain
. t is the intrachain nearest-neighbor transfer and td is the interchain
nearest-neighbor transfer energy. The energy is measured in t units. The energy minimum was given when the components of the gap function k take finite values
plotted in Figure 7 for the lattice of 20 2 sites with 34
electrons imposing the periodic boundary condition . Each component of k was optimized for U08 and
t . There are two characteristic features; one is that the components of the bonding and antibonding bands have opposite signs each other and second is that the absolute values of k of the antibonding band
is much larger than that of the bonding band
. In order to reduce the computation cpu time,
of each band was forced to take a fixed value specific to each band, i.e. 1 for the bonding band and
for the antibonding band. This drastically reduces the number of the variational parameters but still allows us to get a substantial value of the condensation energy.
and 2 take opposite sign, which is similar to that of the dx2y2 gap function.
The energy gain F2c remains finite in the bulk limit
when 1.2 td 1.6. The SC condensation energy per site in the bulk limit is plotted as a function of td in
Figure 8 . The SC region derived from the SC
condensation energy in the bulk limit is consistent with the results obtained from the density-matrix renormali- zation group [55,56] and the exact-diagonalization method [51,52,115]. The maximum value of E2c is
0.0008 which is of the same order of magnitude as the maximum condensation energy obtained for the 2D Hubbard model .
Figure 7. The values of components of k for the two- chain Hubbard model. All the values of k of the bonding x band
ky0 and antibonding band
corre- spond to the energy minimum for 20 × 2 lattice with 34 electrons. The parameters in the Hamiltonian are td 1.8 and U08 and the variational parameters are
Figure 8. t dependence of the SC condensation energy d
2 for the two-chain Hubbard model in the bulk limit .
3.5. Condensation Energy in the d-p Model
The SC energy gain for the d-p model, namely, three- band Hubbard model in Equation (4) has also been evalu- ated using the variational Monte Carlo method. For the three-band model the wave functions are written as
n G k
SC G N k k k k
P P u v
(31) where k is the linear combination of dk , pxk and
p constructed to express the operator for the lowest band (in the hole picture) or the highest band (in the electron picture) of the non-interacting Hamiltonian. The numerical calculations have been done in the hole picture. The Gutzwiller parameter g, effective level difference
, chemical potential and superconducting or- der parameter are the variational parameters.
The similar results to the single-band Hubbard model were obtained as shown in Figure 9 for tpp 0.0,
U and dp2 in tdp units where the cal-
culations were performed in the hole picture . The SC condensation energy for the three-band model is
E t meV per site in the optimally doped region. We set tdp1.5 eV as estimated in Table
1. There is a tendency that Econd increases as dp
increases which is plotted in Figure 10. This tendency is
not, however, in accordance with NQR (nuclear quad- rupole resonance) study on cuprates.  We think that the NQR experiments indicate an importance of the Coulomb interaction on oxygen sites. This will be dis- cussed in Section 3.11.
3.6. Antiferromagnetic State
When the density of doped holes is zero or small, the 2D single-band or three-band Hubbard model takes an anti- ferromganetic state as its ground state. The magnetic
Figure 9. Ground-state energy per site as a function of with the d-wave gap function for the three-band Hubbard model. The size of lattice is 6 × 6. Parameters are U8 ,
t 0 and pd2 in units of t . The doping rate is dp
for (a) and 0.333 for (b). Squares denote the energies for the normal-state wave function .
Figure 10. Energy gain per site in the SC state as a function of the level difference dp pd for the three-band Hubbard model with Ud 8 and tpp0.2 . The size of lattice is 6 × 6 sites.
order is destroyed and superconductivity appears with the increase of doped hole density. The transition between the d-wave SC and the uniform SDW states has been investigated by computing the energy of the SDW state by using the variational Monte Carlo method. The trial SDW wave function is written as
AF PG SDW
SDW u c v c Q u c v c Q
k k k k
k k k k
1 2 2 2
1 AF 2 ,
u w w
k k k (34)
1 2 2 2
1 AF 2 ,
v w w
k k k (35)
w kk (36)
Summation over k and k in Equation (33) is performed over the filled k-points, as in the calculation of the normal state energy. Q is the SDW wave vector given by
, and AF is the SDW potential am- plitude.
As shown in Figure 11, the energy gain per site in the
SDW state rises very sharply from ne0.84 for t 0
. At ne0.84 it is slightly larger than that in the
SC state, and at ne0.80 there is no more stable SDW
state. Thus the boundary between the SDW and the SC states is given at ne0.84. The results of the bulk limit calculations indicate that the energy gain in the SC state at ne 0.84 takes the extremely small value and the
value at ne0.80 vanishes as N0. Hence the pure
d-wave SC state possibly exists near the boundary at
n , but the region of pure SC state is very restricted.
Let us turn to the three-band model. We show the antiferromagnetic-paramagnetic boundary for tpp0.0
and p d 2 in the plane of U and the hole density
in Figure 12 where AF denotes the antiferromagnetic
region . The value p d 2 is taken from the
estimations by cluster calculations [89-91]. The phase boundary in the region of small U is drawn from an extrapolation. For the intermediate values of U8 -12,
Figure 11. Energy gain per site in the SDW state (diamonds) against electron density for t0 and the energy gain in the SC state for t0 (open circles) and t 0.1 (solid circles). The model is the 2D Hubbard model on 10 × 10 lattice .
Figure 12. Antiferromagnetic region in the plane of U and the hole density for tpp0.0 and pd2.
the antiferromagnetic long-range ordering exists up to about 20 percent doping. Thus the similar features are observed compared to the single-band Hubbard model.
Since the three-band Hubbard model contains several parameters, we must examine the parameter dependence of the energy of SDW state. The energy gain ESDW in
the SDW state is shown in Figure 13 as a function of
doping ratio for several values of dp pd. ESDW
increases as dp increases as expected. In Figure 14 pp
t - and Ud -dependencies of ESDW are presented.
The SDW phase extends up to 30 percent doping when
U is large. It follows from the calculations that the SDW region will be reduced if pd and Ud de-
From the calculations for the SDW wave functions, we should set pd and Ud small so that the SDW
phase does not occupy a huge region near half-filling. In
Figures 15 and 16, we show energy gains for both the
SDW and SC states for Ud8, tpp0, 0.2 and
, where the right hand side and left hand side indicate the hole-doped and electron-doped case, res- pectively. Solid symbols indicate the results for 8 8
and open symbols for 6 6 . For this set of parameters the SDW region extends up to 20 percent doping and the pure d-wave phase exists outside of the SDW phase. The
d-wave phase may be possibly identified with supercon- ducting phase in the overdoped region in the high-Tc
3.7. Stripes and Its Coexistence with Superconductivity
Incommensurate magnetic and charge peaks have been observed from the elastic neutron-scattering experiments in the underdoped region of the Nd-doped
Figure 13. Energy gain per site
N in the SDW state as a function of hole density for the three- band Hubbard model. Parameters are tpp0.4 and
U 8 in tdp units. From the top, dp pd3, 2, 1.5 and 1. The results are for 6 × 6, 8 × 8, 10 × 10 and 16 × 12 systems. Antiperiodic and periodic boundary conditions are imposed in x- and y-direction, respectively. Monte Carlo statistical errors are smaller than the size of symbols. Curves are a guide to the eye .
Figure 14. Uniform SDW energy gain per site with reference to the normal-state energy as a function of the hole density for the three-band Hubbard model. Data are from 8 × 8, 10 × 10, 12 × 12 and 16 × 12 systems for
. For solid symbols Ud4 (circles), Ud8 (squares), Ud 12 (triangles) and Ud20 (diamonds) for tpp0.2 . For open symbols Ud8 and tpp0 , and for open squares with slash Ud 8 and tpp0.4 . The lines are a guide to the eye. The Monte Carlo statistical errors are smaller than the size of symbols .
duction is approximately one dimensional . The angle-resolved photo-emission spectroscopy measure- ments also suggested a formation of two sets of one- dimensional Fermi surface . Then it has been proposed that these results might be understood in the framework of the stripe state where holes are doped in the domain wall between the undoped spin-density-wave
Figure 15. Condensation energy per site as a function of hole density for the three-band Hubbard model where
t 0.0 , pd2 and Ud8. Circles and squares denote the energy gain per site with reference to the normal-state energy for d-wave, ext-s wave and SDW states, respectively. For extremely small doping rate, the extended s-wave state is more favorable than the d-wave state. Solid symbols are for 8 × 8 and open symbols are for 6 × 6. Curves are a guide to the eye.
Figure 16. Condensation energy per site as a function of hole density for the three-band Hubbard model where
t 0.2 , pd2 and Ud8 . Circles and squares denote the energy gain per site with reference to the normal-state energy for d-wave and SDW states, res- pectively. Solid symbols are for 8 × 8 and open symbols are for 6 × 6. Curves are a guide to the eye.
, were observed in the SC phase in the range of 0.05 x 0.13 in the elastic and inelastic neutron-scattering experiments with LSCO [127,128,130]. The hole dependence of the incommensurability and the configuration of the spots around the Bragg spot in the SC phase indicated the vertical stripe. The neutron- scattering experiments have also revealed that a diagonal spin modulation occurs across the insulating spin-glass phase in La2–xSrxCuO4 for 0.02 x 0.05 , where a one-dimensional modulation is rotated by 45 degrees from the stripe in the SC phase. The incommensurability
versus hole density is shown in Figure 18 sche-
matically [129,130]. The diagonal stripe changes into the vertical stripe across the boundary between the insulating and SC phase.
Let us investigate the doped system from the point of modulated spin structures [131-141]. The stripe SDW state has been studied theoretically by using the mean- filed theory [132-136]. They found that the stripe state appears when an incommensurate nesting becomes
Figure 17. Charge and spin density as a function of the distance for a striped state .
Figure 18. Schematic illustration of the incommensurability versus hole density.
favorable in the hole-doped 2D Hubbard model. When the electron correlation correlation is strong or inter- mediate, it was shown that the stripe state is more stable than the commensurate spin-density-wave state with the wave vector
, in the ground state of the 2D Hubbard model by using the variational Monte Carlo method . It has also been confirmed by the same means that the stripe states are stabilized in the d-p
model . The purpose of this section is to examine whether the superconductivity can coexist with static stripes in the 2D Hubbard model in a wider doping region and investigate the doping dependence of the coexisting state.
We consider the 2D Hubbard model on a square lattice. We calculate the variational energy in the coexistent state that is defined by
e MF coexist P PN G coexist
(37) where MF
is a mean-field wave function. The effective mean-field Hamiltonian for the coexisting state is  represented by
† , ij
MF i i
ij ji ji j
H F c
H c c
F H c
where the diagonal terms describe the incommensurate spin-density wave state:
sign 1 ,
ij ij i i ij
H t n m (39) where is the chemical potential. The vertical stripe state is represented by the charge density ni and the
spin density mi that are spatially modulated as
1 cosh i ,
c y Y
tanh i ,
c y Y
where Y denotes the position of vertical stripes. The
amplitude is fixed by
ini Ne. The off-diagonal
terms in Equation (38) are defined in terms of the d-wave SC gap as
ij ij ji e
where ˆe xˆ, yˆ (unit vectors). We consider two types of the spatially inhomogeneous superconductivity: anti-phase and in-phase defined as
. cos ,
i i x q yy i Y
, cos ˆ 2 ,
i i y q yy i Y y
. cos ,
i i x q yy i Y
, cos ˆ 2 ,
i i y q yy i Y y
respectively. Here, q
and is a in-
commensurability given by the stripe’s periodicity in the
y direction with regard to the spin. The anti-phase (in- phase) means that the sign if the superconducting gap is (is not) changed between nearest domain walls.
The wave function 0
is made from the solution of the Bogoliubov-de Gennes equation represented by
ij j ij j
H u F v E u
ji j ji j
F u H v E v
(48) The Bogoliubov quasiparticle operators are written in the form
i i i i
u c v c E
i i i i
u c v c E
(50) Then the coexistence wave function is written as [105,142]
e coexist N
N ij i j
i j ij ij
CP U V c c
C U V c c
for constants C and C . The calculations are performed for the wave function 0
coexist PG coexist
variational parameters are , m, g, c and s. The
system parameters were chosen as t 0.20 and 8
U suitable for cuprate superconductors. It has been shown that the “anti-phase” configuration is more stable than the “in-phase” one .
Here, the system parameters are t 0.2 and U8. We use the periodic boundary condition in the x-di- rection and anti-periodic one in the y-direction. In Figure 19, we show the total energy of the coexistent state,
E , as a function of the SC gap for the cases of anti-phase and in-phase. The SC condensation energy
is estimated as 0.0008 t per site at the hole density 0.125 on the 12 8 lattice with periodic boundary condition in x-direction and antiperiodic one in
y-direction. Ecoexist in the coexistence state is defined
as the decrease of energy due to finite . If we use
t , this is evaluated as 0.4 meV. The SC condensation energy per site is shown as a function of
hole density in Figure 20. One finds that Ecoexist in the
stripe state decreases as the hole density decreases. This tendency is reasonable since the SC order is weakened in the domain of the incommensurate SDW because of the vanishingly small carrier concentration contributing the superconductivity in this domain. This behavior is con- sistent with the SC condensation energy estimated from the specific heat measurements .
There is a large renormalization of the Fermi surface due to the correlation effect in the striped state . We considered the next-nearest transfer t in the trial function as a variational parameter t. In Figure 21,
Figure 19. Coexistent state energy per site Ecoexist Ns versus for the case of 84 electrons on 12 × 8 sites with
U8 and t 0.2 . Here the vertical stripe state has 8-lattice periodicity for the hole density p0.125 . Only
E N for the optimized gap is plotted for the in-phase superconductivity.
Figure 20. Superconducting condensation energy per site in the coexistence state as a function of the hole density
Figure 21. Optimized effective second neighbor transfer energy t t as a function of U t . The system is a 16 × 16 lattice with t t 0.2 and the electron density 0.875.
optimized values of t t for the striped state are shown as a function of U t . The t t increases as U t increases. We also mention that the optimized t t
almost vanishes. The renormalized Fermi surface of 0.30
t t , 0.40 and 0.50 are plotted in Figure
22. The system is a 16 16 lattice with t t 0.2 and
the electron density 0.875. As U t is incresed, the Fermi surface is more deformed. We show the the gradient of the momentum distribution function, nk ,
calculated in the optimized stripe state in Figure 23. The
brighter areas coincide with the renormalized Fermi surface with t t 0.31 and t t 0.0 for U t8.
The calculations for the three-band Hubbard model has also been done taking into account the coexistence of stripes and SC [15,106]. The energy of antiferromagnetic state would be lowered further if we consider the incom- mensurate spin correlation in the wave function. The phase diagram in Figure 24 presents the region of stable
AF phase in the plane of tpp and dp pd. For large dp pd, we have the region of the AF state
with an eight-lattice periodicity in accordance with the results of neutron-scattering measurements [118,123]. The energy at x1 16 is shown in Figure 25 where the
4-lattice stripe state has higher energy than that for 8-lattice stripe for all the values of tpp.
The Bogoliubov-de Gennes equation is extended to the case of three orbitals d, px and py.
Fij are now 3N3N matrices. The energy of the
state with double order parameters and m is shown in Figure 26 on the 16 4 lattice at the doping rate 1/8.
The SC condensation energy per site is evaluated as 0.00016tdp
for Ud 8, tpp0.4 and p d 2. If we use tdp1.5 eV [89-91], we obtain Ecoexist
0.24 meV which is slightly smaller than and close to the value obtained for the single-band Hubbard model. We show the size dependence of the SC condensation
Figure 22. Renormalized quasi-Fermi surface for
t t 0.3 , 0.4 and 0.5 . The system is the same as that in Figure 21.
Figure 23. Contour plot of nk measured for the pro- jected stripe state on 24 × 24 lattice with t t 0.2. The electron density is 0.875.
Figure 25. Energy as a function of tpp for 16 × 16 square lattice at x1 16. Circles, triangles and squares denote the energy for 4-lattice stripes, 8-lattice stripes, and commensurate SDW, respectively, where n-lattice stripe is the incommensurate state with one stripe per n ladders. The boundary conditions are antiperiodic in x-direction and periodic in y-direction [47,106].
Figure 26. Energy of the coexistent state as a function of the SC order parameter for x0.125 on 16 × 4 lattice. We assume the incommensurate antiferromagnetic order (stripe). Parameters are p0, d 2, tpp0.4 and
U 8 in tdp units. For solid circles the SC gap function is taken as i i x,ˆ cos
i iy Qx xi
, cos , while for the open circles
i i x Qx xi x
, cos 2 and i i,ˆy cos
Q 2 4.
energy for x0.2, 0.125 0.08333 and 0.0625 in Figure 27. We set the parameters as p d 2 and tpp0.4
in tdp units, which is reasonable from the viewpoint of
the density of states and is remarkably in accordance with cluster estimations [89-91], and also in the region of eight-lattice periodicity at x1 8. We have carried out the Monte Carlo calculations up to 16 16 sites (768 atoms in total). In the overdoped region in the range of 0.18 x 0.28, we have the uniform d-wave pairing state as the ground state. The periodicity of spatial
variation increases as the doping rate x decreases pro- portional to 1x. In the figure we have the 12-lattice periodicity at x0.08333 and 16-lattice periodicity at
x . For x0.2, 0.125 and 0.08333, the results strongly suggest a finite condensation energy in the bulk limit. The SC condensation energy obtained on the basis of specific heat measurements agrees well with the variational Monte Carlo computations . In general, the Monte Carlo statistical errors are much larger than those for the single-band Hubbard model. The large number of Monte Carlo steps (more than 5.0 10 7) is required to get convergent expectation values for each set of parameters.
In Figure 28 the order parameters AF and SC
Figure 27. Energy gain due to the SC order parameter as a function of the system size Natom 3Ns. Parameters are
, d 2, tpp 0.4 and Ud8. The open circle is for the simple d-wave pairing at the hole density x0.2 . The solid symbols indicate the energy gain of the coexistent state; the solid circle is at x0.125 , the solid square is at x0.08333 and the solid triangle is at x0.0625 . The diamond shows the SC condensation energy obtained on the basis of specific heat measurements .